advertisement

Pergamon

Acta mazer. Vol. 45, No. 11, pp. 45614568, 1997

0 1997 Acta Metallurgica Inc.

PII: s1359-6454(97)-00125-o

Published bv Elsevier Science Ltd. All rights reserved

Printed in &eat Britain

**K. **

BHATTACHARYA’T, R. D. JAMES* and P. J. SWART’

‘Division of Engineering and Applied Science, 104-44 California Institute of Technology, Pasadena,

CA 91125, ‘Department of Aerospace Engineering and Mechanics, University of Minnesota, Minneapolis,

MN 55455, and ‘Theoretical Division, MS-B284, Los Alamos National Laboratory, Los Alamos,

NM 87545,

**U.S.A. **

*(Received 12 November 1996; accepted 27 March 1997) *

**Abstract-A **

variety of relaxation phenomena such as stabilization of martensite, rubber-like behavior, evolving hysteresis loops and stabilization of interfaces have been observed in various shape-memory alloys. These effects adversely impact technological applications. In Part I of this paper we proposed a phenomenological, but predictive, model of the mechanical behavior of these materials. We showed that this model reproduces the experimental observations. In this part, we extend this model to include the effects of temperature and the austenite-martensite transformation. Once again, the predictions from this extended model agree with experimental observations. We can therefore conclude that the basic phenomenological ideas combined with a few easily measured material parameters is sufficient to predict the behavior of these materials. Finally, we propose new experiments in order to probe longstanding issues concerning the mechanism responsible for the relaxation. c 1997

*Acta Metallurgica Inc. *

**1. INTRODUCTION **

*2. *

**STABILIZATION OF MARTENSITE **

A variety of relaxation phenomena such as stabiliz- ation of martensite, rubber-like behavior, evolving hysteresis loops and stabilization of interfaces have been observed in various shape-memory alloys. These effects adversely impact technological applications.

In Part I [1] of this paper (henceforth referred to as

Part I) we proposed a phenomenological, but predictive, model of the mechanical behavior of these materials. The model and the important material parameters are summarized at the end of Section 4 in that paper. In Section 2 below, we extend the model to include temperature changes and the austenitee martensite transformation. In particular, we examine the effect of various thermomechanical the migration of the austenite-martensite ation temperature. histories on transform-

We show that the predictions agree with experimental observations. Finally, we use the model in Section 3 to design new experiments in

In this section we extend the energy introduced in

Section 3 of Part I to temperatures above the martensitic transformation temperature. We write down an energy suitable for a material undergoing transformation from a high temperature “austenite” phase to a low temperature “martensite” phase with two variants, “ + ” and “ - “. The austenite has preferred strain and shift (0, 0} while the martensite variants have preferred strain and shift {t+, I} and

{EC, - l}, with C+ > 0 > CC. We assume the existence of a temperature O0 such that the free

*energy per unit reference volume cp(t, p, 0) *

satisfies cp(O,O, 0) < (P(GP, 0) if 0 > 00,

(P(t+, l, 0) = cp(c-, - l, Q) < (P(GP, 0) if 19<&.

We do all our calculations with the energy

(2.1) order to further concerning understand the mechanism relaxation. longstanding responsible issues for the which is the minimum of three quadratic whose depths depend linearly on temperature. define wells

We tTo whom all correspondence should be addressed. i” = i, - 1,;

(2.3)

4561

4562

BHATTACHARYA ef al.: SHAPE-MEMORY ALLOYS-II

L is the latent heat of transformation and we assume that it is positive. Notice that we have assumed for simplicity that the moduli are the same for the austenite as well as for both the variants of martensite.

As in Part I, we shall use

*D = 6/a *

(respectively,

*a, B = ,t? - d2[a *

the elastic modulus, and the normalized shift modulus and the normalized coupling modulus) as the material parameters to be determined c+

9 c- from experiment. rather

ET = E+ + c + 20. than

However, we retain combining them in

Assume that the bar is immersed in a heat bath of temperature e(t) and subject to an applied load F(t). As in Part I, equation (3.6), we let a(x, t) = F(t)/A(x) and define the total energy by,

- a(x, t)c(x, t)} dx.

(2.4)

Note that we have implicitly assumed that the temperature is uniform in the bar and is equal to the temperature of the heat bath at each time.

This is reasonable if the time required for the bar to attain thermal equilibrium is much smaller than the typical processes (relaxation) that we wish to study.

Based on this energy we write down a model analogous to that of Part I, Section 4. There, we wrote down a model based on energy minimiza- tion, but then slightly modified it by adding an

“inherent section we hysteresis” 6,. For simplicity, in this confine ourselves to the energy minimization not add inherent hysteresis.

L

(i) min

= 0 i o

-&){cp(ck

(3

- a(x, t)~(x, t)} dx

$

(x7 4 =

-P t)*P(x, Q,~(t)) at each t,

$

(4x, t),p(x, t), e(t)>, and do

For a prescribed load F(t), temperature e(t) and initial distribution of shift p,,(x) and strain co(x), the functions u(x, t) and p(x, t) are determined by

(iii) p(x, 0) = pa(x), E(X, 0) = co(x), 0 < x <

*L. *

*(2.5) *

Here, as before, the minimization p > 0 is the mobility, problem is interpreted and as in

Part I.

We now specialize to the energy (2.2) and describe the solution procedure, which is analogous to that of Section 4 of Part I. We begin with (2.5) for a given t and p(x, t). In order to minimize the total energy, we choose a strain that minimizes the integrand and x, we at each x. Thus, for a given choose

6(X, t) to minimize t f(c) = q(c,p(x, t), e(t)) - u(x, t)~. Since, cp has a triple-well structure, the equation (drp/&) = 0 has three solutions: c = c- + o/a -

*[email protected] + I) *

E = .c+ +

*o/a - D(p - *

and E = a/a -

*Dp. *

l),

By com- paring the values off on these three solutions we conclude that c- + q - [email protected](x, t) + 1) if

*c(x,t)= c+ + +$ - *

[email protected](x, t) -

1) if

*9 - *

*Dp(x, t) if {P(x, 0,4x, t), w)) E @, *

*(2.6) *

where

W-=

*{p,a,O}: a< -yp *

and @-- w+= {p,a,ej:

02 -yp and

*B 1-p *

*[(A *

*-6(6++D) *

11 w”=

{P,d}:

**! **

and

(e-eo)a

-i

**[( > - **

D)

1

*-:[B(;-p)--o(s-+D)] *

(2.7)

BHATTACHARYA et al.: SHAPE-MEMORY ALLOYS-II and y = 2BIcr is defined as in Part I

*(cf. *

equation

(4.4)).

For a fixed (T, the regions W-, W+ and @ are shown in Fig. I. The 8-p plane is divided into the 3 regions by a horizontal “Y”. First look at the low temperatures. Here, we are either in W+ or %’ so according to (2.6), the strains are either close to C+ or t- and the material is either in the + variant or - variant of martensite. The exchange of stability takes place when p = -(l/r)a, i.e., when cs = -7~. In other words, at low temperatures, when the stress is above the Maxwell

*stress, *

the material is in the + variant of martensite and when the stress is below the

Maxwell stress, the material is in the - variant of martensite. This is exactly as in Part I, Section 4; in particular, the Maxwell stress depends on the shift.

At high temperature @, g, 0) is in the region w”, the strains are close to 0 and the material is in the austenite phase. The exchange of stability between the austenite and the two variants of martensite takes place along the two arms of the horizontal Y so that the transformation temperature depends both on the stress and the value of the shift. The slopes of these arms are given by

**(A/B). *

The latent heat n(0) determines the change of transformation temperature due to both shift and stress, while the parameter

*B/i *

determines the effect of shift on transition tempera- ture at constant stress. Notice that depending on the value of the shift, the austenite loses its stability to one or the other variant of martensite. Finally, the horizontal Y moves up with decreasing o and down with increasing a; it also moves sideways and the direction of the motion depends on the sign of fJ(c+ + CC).

We now turn to (2.5)i. Using (2.2) and (2.6) we obtain

E

**: **

e a

,m

$

**E **

**2 **

**330 **

**310 **

**0 **

**400 **

**I **

**800 **

**Ageing Time (Mins) **

**1 **

**1200 1600 **

Fig. 2. The stabilization of martensite. The

*A, *

temperature of a bar held in the martensite state rises with holding time.

The diamonds show the experimental results extracted from

Murakami et al.

[3], while the curve is the prediction, according to the model and parameters (2.15).

We integrate

.

I

(2.Q1 using a procedure similar to Part I, Section 4.

To illustrate, let us fix x and suppress it from the notation.

+ d ‘a(s)e~“~‘- 7, ds. s 0

(2.9)

We continue with this solution until the first time at which (p(t,), a(t,), O(t,)} hits the boundary of %. t,

Suppose it hits the boundary between B- and %?+. At

*t = tl, we *

switch to the + branch, (2.8),,. Integrating

(2.8),i with the initial condition

*p+(t,) = p(t,) = p,, we get p(t) = p’(t) = *

1 + (p, - l)e-m(‘- ‘1)

+ d

,

Suppose (pO, a(O), 0(O)} E g-. we integrate (2.8) to obtain p(t) = p-(r) = - 1 + (Jo + I),-,(‘-0’

.

4563

(2.8) subject to the initial conditions

Therefore,

(2.10) g (x, t) =

-mMx, t) +

1) + [email protected], t) if

(p(x, t), 4x, t), e(t)}

E

W-

-mGo(x, t) - 1) + [email protected], t) if

*-mp(x, t) + da(x, t) *

{p(x, t), 0(x,

*t), e(t)} E .c%+’ if {Ax, t), a(~, t), e(t)} E * *

*(2.8) *

where m =

*pB *

and

*d = -pD *

as in Part I, Section 4.

We continue with this solution until the first time tz at which

{p(h), a(h), O(h)} hits the boundary of a+.

Suppose it hits the boundary between &?+ and @. At t = t2, we switch to the austenite branch, (2.8),,,.

Integrating (2.8),,, with the initial condition p”(tz) = p(h) = ~2, we get p(t)

*=p”(t) =p2emm(‘+‘2) + *

d

‘o(s)e-““-y’ds. s

12

(2.11)

Fig. 1. Regions of stability of the austenite and the “ + ” and “ _ ” variants of martensite in the o-p plane. Note that

Q(u) = eo - (1/21)[8 - fr(t+ + t-)].

We continue at which with this solution

{p(h), CT until the first time t, hits the boundary of L%‘.

Depending on which boundary it hits, we continue the solution on the relevant branch and so on. low an

We fol- analogous procedure if {p,,, a(O), 0(O)] is in

4564 BHATTACHARYA

*et al.: *

SHAPE-MEMORY ALLOYS-II

W- or R”. Repeating this procedure for each point x, we obtain p(x, t). Substituting this back in (2.6) we obtain 6(x, t) and then, by integration, the displace- ment u(x, t).

We now apply this model to a few simple problems. in both parts of the bar. Since

*B, 1 > 0, *

the reverse transformation temperature increases with holding time in agreement with experimental observations.

(See the paragraph following (2.7) for a discussion of the parameter

*(B/A).) *

Indeed, for the values

*Stabilization of thermal martensite *

Consider a stress-free bar which has been aged in the austenite phase and quenched to a temperature where it completely transforms to the martensite.

Suppose it is held at this temperature for a period of time t*.

It has been observed in many common shape-memory alloys subjected to the above treat ment that the reverse transformation increases with holding time t*. temperature A,

In particular, the diamonds in Fig. 2 are the experimental extracted from Murakami

*et al. *

data

[3] in Au_49S%Cd alloy (note that the composition of this alloy is different from that studied earlier). This phenomenon is called the stabilization of martensite important technological implications. and has

We now examine this problem with our model. We consider a bar with uniform cross-section A in the aged austenite so that the shift p = 0 at each point.

Before we prescribe initial conditions and applied temperature, let us first examine the transformation temperature e,(O) for this aged bar when the applied stress is zero. Setting

*p = 0, u = 0, *

it is clear from either (2.7) or Fig. 1, that the austenite loses its stability on w”) when the temperature

*e=e,(o)=e,-~. *

Further, it loses its stability to both variants of martensite. In other words, when p = 0, c = 0 and

0 < e,(O), both variants of martensite are stable.

Thus, on quenching an aged bar, we expect a part I+ to transform to the + variant of martensite and the remaining part I_ to transform to the - variant.

Therefore, we start with initial data PO(X) = 0,

G,(X) = c+ +

*D *

t,,(x) = t- -

*D *

for for x E

*I_ *

x E

*1, *

and corresponding

*PO(X) = 0, *

to an aged and quenched bar. The applied stress is zero and the applied temperature is constant at 8, (where

8, < e,(O)).

Now, for

*t > 0, we *

integrate (2.8)ii for x E

*I+ *

and

(2.8) for x E

*l_ *

to obtain

Notice that since c = 0 and remain in the + variant and similarly remain in the - variant.

At time t = t*, the value of the shift has evolved to

*p+(t*) *

in

*1, *

and p-(t*) in

*I-. *

Therefore, according to

(2.7), the transformation

*B p+ > 0, 1, *

=;I.

(2.12)

(2.13) continues to

*I_ *

continues to temperature changes to

0 = &(t*) = B,, - 5 + f (1 - eem”) (2.14) we obtain

00 = 319.66 K,

*B/A = m = *

18.12 K,

0.009465 min-‘, the curve shown in Fig. 2, in good agreement with experimental observations.

(2.15)

*Mechanical destabilization of the stabilized thermal martensite *

Consider an aged bar of the austenite phase.

Suppose it is quenched to a temperature 0, < & -

B/(U) where it completely transforms to a mixture of martensite variants. Suppose it is held at that temperature at zero load for time t*.

As we have seen above, the martensite begins to stabilize as the shift evolves according to (2.13) to

*p+(t*) *

in

*1, *

(the part of the bar that transforms to the + variant) and

*p-(t*) *

in

*I_. *

Furthermore, as we have seen in (2.14), the reverse transformation temperature rises to

&(t*) indicating a stabilization of the martensite.

Suppose at time

*t = t*, we *

begin to apply a sinusoidal load F(t) =

*F0 *

sin(o(t - t*)) (with

*Fo *

chosen large enough to detwin the bar), while still maintaining the temperature constant at 8,. Since the temperature temperature, is constant below the transformation we involve only the two variants of martensite. In other words, for t > t*, this problem is exactly the one studied extensively in Part I, Section

4. It is clear from Fig. 4 there that with increasing cycles of the applied load, the value of the shift in both parts

*1, *

and

*l_ *

of the bar begins to approach zero and after a sufficiently large number of loading cycles, the shift is very close to zero in the entire bar,

Therefore, after this loading, the (reverse) transform- ation temperature is going to be close to &(O) (the transformation is smaller than loading, temperature of aged austenite) which

&(t*). we have

Thus, by applying a sinusoidal been able to decrease the transformation temperature, i.e., we have been able to (mechanically) destabilize the (thermally) stabil- ized martensite.

Let us discuss this prediction in the light of our one-dimensional three-dimensional hypothesis. First note that in a full theory, which is difficult to construct at this time because of the lack of knowledge of the precise mechanism, we would need to allow for vector-valued shifts. Then it is not clear that cycling between two variants of martensite would cause the shift to evolve to the preferred value of the austenite. However, symmetry considerations suggest that qualitative aspects of this prediction should still be true. If, as is the case in many martensitic transformations, the point group of the martensite is a subgroup of that of the austenite, then,

BHATTACHARYA et al.: SHAPE-MEMORY ALLOYS-II

4565 the preferred values of the shifts for the different variants of martensite are likely to be related by the action of this group. If the austenite has cubic symmetry, for example, this implies that the preferred values of the shifts for the different variants of martensite lie on the corners of a regular polyhedron centered at the origin, while the preferred shift for austenite is zero. Furthermore, cycling between two variants would cause the shift to evolve to an average value which would be closer to the center (preferred value of austenite) than the corners. Thus we expect that during cycling the shift will evolve toward the preferred value(s) for austenite and, consequently, the transformation temperature should decrease, though not possibly to the value for aged austenite. Hence, measurements of the three temperatures: e,(O), &(t*) and the transformation temperature extensive cycling of the martensite, just after will provide indirect information about the mechanism; if the two latter temperatures are nearly equal, it suggests that the ordering or shuffle that develops after long term cycling of the martensite is close to that of the aged austenite.

Based on these considerations, we suggest this as an experiment to examine whether the mechanism responsible for the stabilization of martensite is the same one responsible for the rubber-like behavior.

*Stabilization *

*qf *

*stress-induced martensite *

Consider a bar with uniform cross-section A aged in the austenite state. Suppose we continue to hold this bar at a constant transformation temperature temperature above the and subject it to an applied stress g* large enough so that the bar fully transforms to the martensite. We hold this load for time t* and seek the state of the bar. In particular, we seek to know if the bar would revert to the austenite when unloaded; if so, we seek the value of applied stress at which the reverse transformation takes place. Finally, if the bar is unloaded at time t* and reverts to the austenite, we seek the temperature at which it would transform to the martensite on sudden cooling.

Before we prescribe the initial data, let us examine the transformation stress for a bar aged in the austenite state. We take

*p = 0 *

and applied tempera- ture 0 > 0,(O) = B0 - (B/U) (cJ (2.12)). For these values, it follows from (2.7) that the austenite transforms to + and - variants at the stress

In other words, if we apply a tensile stress larger that o+(O), the austenite transforms to the + variant while if we apply a compressive stress larger than lam(O the austenite transforms to the - variant. In particular, we note the interesting relationship a+(f*) =

((+

**~{H-(Bo-$)} **

+

D) o-(O)t+ z C(O)CC.

We note in passing that in this one-dimensional theory, there is no kinematic compatibility. In three dimensions, kinematic compatibility crystallographic

(written as the theory of martensite, for example) would prevent the austenite from transforming to a single variant of martensite. So in reality we would expect the austenite to transform to a mixture of the two variants and then to a single variant. In any case, what (2.16) says is that it is possible to stress-induce the martensite and that the + and - variants are stable when we apply sufficiently large tensile and compressive stresses respectively.

We now return to the problem of the bar aged in austenite. We apply a constant temperature

(3 > &, - (B/21) g* > a+(O). We and a constant choose initial applied data stress

*p. = 0, co = t+ + a*/~ + D *

for each x in the bar correspond- ing to aged austenite freshly transformed to the + variant of martensite under the action of the applied stress. For time

*t > 0, p(x, t) *

evolves according to equation (2.Q (which corresponds to the + variant).

Integrating it with the initial conditionp, = 0, we find that for each x in the bar,

*p(x, t) = p*(t) = *

1 + (0 - 1)e +’

+ d ‘a(s)e-“(‘-‘) ds s cl

(1 - e-“‘).

(2.17)

(2.18)

At time

*p*(t*) *

t = t*, the shift has evolved to the value and consequently according to (2.7) the stress for reverse transformation is given by

(1 - em”“*). (2.19) and a+(O) =

00) =

**&j{+S)i **

**-{Q-(8,-$-)}, **

(cm

‘-

D)

(2.16) respectively. Since we have assumed that E+ > 0 > c-

Thus, we see that stress for reverse transformation o+(t*) changes exponentially with holding time.

Further, the stress may increase or decrease depending on the value of (1 - Do*/@. In particular, if D < 0, the stress increases with holding time.

Finally suppose the bar is unloaded at time t = t* and reverts to the austenite. transformation temperature

We examine the if the bar is suddenly cooled at time is given by t = t* p*(t*),

+ . Since the value of the shift the transformation temperature

4566 changes to

BHATTACHARYA et

*al.: *

SHAPE-MEMORY ALLOYS-II e = B&t*) =

& - $ + f (1 - Do*/B)(l - e-m’*). (2.20)

Thus, depending on the sign of

*D *

and the magnitude of the applied load, the stress-induced martensite is either stabilized or destabilized. difference compared

This is a key with the thermal martensite where the martensite is always stabilized (cJ (2.14)).

**3 **

**2 **

**1 **

**I44 **

0’

0

**3 **

**2 **

**1 **

0”

0

(b) cl

**3. **

0.01 r

0

**2 **

**I. **

**.-.__I **

(4

0.01 z

(4

Fig.

4. Simulated hysteresis (stress vs overall strain) with loading (3. 2) with

*Fo/A = 3.1 *

and w = 7.5 x 10-2Hz and material parameters (3.3). (a) Initial loop, (b) loop after 100 cycles (c) terminal loop after 1000 cycles.

3. PROPOSALS

FOR NEW EXPERIMENTS

In this section, we propose some new experiments to (a) critically examine our theory and (b) to use our theory to explore the mechanism responsible for the relaxation.

*Mechanical tests *

Lieberman

*et al. *

[2] were interested in the behavior of the material under both tension and compression.

Consequently, nonuniform they were forced to use a severely cross-section in order to prevent buckling. Further, they measured the diametral strain and converted it to actual strain. Unfortunately, this introduces various complications liable material parameters. in extracting re-

Therefore, we propose using a specimen with uniform cross-section. The loading programs below are limited to tension; so buckling is not a concern. Further, we suggest that the actual extension be measured directly using a suitable extensometer.

Consider a single crystal bar of austenite. Cool it carefully to transform it to the martensite using a single austenite-martensite interface to obtain a fairly uniform distribution of fine twins of two variants of martensite. Age the bar in this state and then subject it to the various experiments described below. It is important to start each experiment with an aged finely twinned bar.

1.

*Load-hold-unload. *

experiment parameters: in order

We begin with a very simple to determine the material

First measure

OM

%l the volume fractions of the two variants in the aged finely twinned bar. Apply a tensile load large enough so that one of the two variants (the one with initial volume fraction 2) completely disappears. Hold the load constant at this value for a time t* and then unload to zero. Repeat this experiment with different holding times, taking care to start with an aged bar on each occasion.

We expect to obtain a hysteresis loop of the type shown schematically in Fig. 3. We expect CI, QY, EM to remain constant independent of holding time t*, while u, and cg are expected to change with holding time t*.

The parameters may be obtained from the following formulas: cr, = c, + [email protected]‘* for some constants cl and c2,

Cc=

*6x3 = (b&f - cm II’ = [email protected], *

*B = cr(bu - a,>/?, *

(y+ZL)(l

(3.1)

The first three equations give ET, cr,,

*B *

respectively, the fourth gives

2.

*m = -pB, *

*Tension cycle, *

and the fifth gives

Apply a load

*D. *

F(t) =

FoIsin(27rwt)l

(3.2) for F. >

*[(B/CT) + o,]A *

where A is the cross-sectional area of the bar (since we will plot only stress, we do not need the value of A).

In the initial cycles, our model predicts a hysteresis loop like the one shown in Fig. 4(a). With cycling, the hysteresis loop begins to come down as in Fig. 4(b).

After a sufficient number of cycles, the hysteresis loop completely disappears and the bar behaves almost like a linear elastic bar as shown in Fig. 4(c). These curves were simulated using the parameters

CI = 3000 kg/mm2,

*B = *

0.017 kg/mm’,

*D = *

-0.003 kg/mm2,

(3.3)

Fig. 3. A schematic hysteresis loop (stress vs overall strain) during the load-hold-unload test.

ET = 0.02,

BHATTACHARYA et al.: SHAPE-MEMORY ALLOYS-II 4567 oxs = 0.2 kg/mm2, p = 0.8 mm2/(kg min), which are the same as those for equation (6.3) in Part

I. Clearly, the experimental results must be compared with curves simulated using the parameters deter- mined by the load-hold-unload experiment and (3.1).

Once the bar is in the terminal loop, stop the loading at zero load and hold for time t*. Then resume the loading (3.2). Our models predict that the stress-strain curves will remain similar to the collapsed terminal loop shown in Fig. 4(c); if the parameter

*D *

is negative experiments of Lieberman

(as suggested by the

*et al.), *

the stress-strain curve will shift slightly to the left. In any case, our model predicts that under the tensile loading (3.2) there will not be any recovery like that observed by

Lieberman

*et al. *

[2] (see Fig. 1 of Part I).

Repeat the experiment of tensile cycling of an aged finely twinned bar at different temperatures as well as different frequencies and amplitudes of loading. Our model predicts that the hysteresis loops will qualitatively look similar to those shown in Fig. 4.

The width of the initial hysteresis loop is predicted to increase with increasing temperature, decreasing frequency prediction and increasing amplitude (this last will be true if the material parameter

*D < 0, *

but will be reversed if

*D > 0). *

3.

*Unusual tension cycle. *

Apply a load completely disappear; instead it attains the terminal loop as shown in Fig. 5(c). Further cycling does not cause any changes. Note that these figures were generated using parameters (3.3). Clearly, the experimental results must be compared with curves simulated using the parameters determined by the load-hold-unload experiment and (3.1).

Once the bar is in the terminal loop, stop the loading at zero load and hold for time t*. Then resume the loading (3.3). Our models predict that with increasing holding time t*, the hysteresis loop gradually recovers, in contrast with the previous experiment; with sufficiently long holding time it completely goes back to the initial loop.

4.

*Effect of orientation. *

load-hold-unload for

Repeat Experiment specimens with

1, different orientation and determine depend on orientation. how the parameters

It is likely that different mechanisms orientation of relaxation dependence will predict different of the parameters. This information mechanisms, for the models. may prove crucial for testing different and would provide useful guidelines development of 3D shift relaxation

*Thermal and combined thermal-mechanical tests *

An important question is whether the mechanisms responsible for the rubber-like behavior and stabiliz- ation of martensite are the same. In Section 2, we presented a theory assuming that they were the

*same. *

*F0 *

sin(2nwt) if n < t < w if [ for some F. > [(B/cr) + o,,]A cross-sectional where A is the area of the bar. This loading cycle consists of a tension cycle of duration l/30 followed by a hold at zero load for a duration of 2130.

In the initial cycles, our model predicts a hysteresis loop like the one shown in Fig. 5(a). With cycling, the hysteresis loop begins to come down as in Fig. 5(b).

However, unlike Fig. 4, the hysteresis loop does not

0.01 e

**0.01 p **

0.01 z

(4 (b)

(6

Fig.

5. Simulated with loading hysteresis

(3.4) with loops (stress vs overall strain)

*Fo/A = 3.1 *

and w = 7.5 x 1O-2 Hz and material parameters (3.3). (a) Initial loop, (b) loop after

200 cycles and (c) terminal loop after 1000 cycles.

Based on this theory we proposed and predicted the results of three sets of experiments; we collect them here.

5.

*Stabilization of thermal martensite. *

single crystal bar of austenite.

Consider a

Cool it until it completely transforms to martensite. Hold it in the martensite for time t*. Heat it and measure the temperature at which it transforms to the austenite

(either A, or A, will do as long as it is used consistently). Repeat the experiment with different holding times. We expect that the transformation temperature will increase with t* according to the relation (2.14). From the data, we can easily obtain

*B/A *

and

*m. *

From an independent of latent heat 1 we can obtain measurement the parameters

*B *

and p =

*m/B. *

values obtained

Compare these values with the from the mechanical tests (3.1).

If they are similar, then the mechanisms responsible for the rubber-like behavior and stabilization of martensite are likely to be the same. On the other hand, if they are not similar, it is a strong evidence that the mechanisms are different.

4568

BHATTACHARYA

*et al.: *

SHAPE-MEMORY ALLOYS-II

6.

*Mechanical thermal martensite. destabilization of the stabilized *

Consider a single crystal bar of austenite. Cool it until it completely transforms to martensite. Hold it in an unloaded state in the martensite for time t*. At time t = t*, subject the bar to a sinusoidal tension-compression loading cycle similar to those considered by Lieberman

*et al. *

[2] and considered in length in Sections 4, 5 and 6 of Part

I. Notice that this experiment may require care to prevent buckling. Initially the hysteresis response will be a double loop; with cycling it will evolve to the terminal single loop. Once the specimen attains the terminal loop, stop the loading and heat until it transforms to the austenite and measure the transformation temperature. Our one-dimensional model predicts that the transformation will be independent of the holding time temperature t*; however, as we noted in Section 2, this prediction may depend crucially on the exact three-dimensional nature of the mechanism and the underlying material symmetry.

Therefore, information ism. this experiment may provide critical about the nature of the exact mechan-

7.

*Stabilization of stress-induced martensite. *

Con- sider a single crystal bar of austenite. Apply a tensile load until it fully transforms to the martensite. Hold the load for a time t* and then unload. Measure the value of the load at which it transforms back to the austenite. Our model predicts that this will depend on the holding time according to (2.19); therefore we can estimate the coupling parameter

*D *

and contrast it with that obtained from the purely mechanical tests.

4. CONCLUSION AND DISCUSSION

A wide variety of relaxation phenomena like the stabilization of martensite and rubber-like behavior are known to occur in common shape-memory alloys.

These phenomena adversely affect applications.

There is a great wealth of experimental data; yet there is no agreement on the exact mechanism. However, there is a broad consensus that “the free energy per unit volume in the region swept by the moving twin boundary is temporarily increased but may be decreased again by some thermally activated relax- ation process” (Christian [4]).

We have proposed a phenomenological, but predictive, model of the behavior of these materials based on this point of view. The basic model was presented in Part I and extended to include temperature in Section 2 of this part. The model is one-dimensional and is based on an energy which depends on strain and an internal variable which we call shift. Section 2 of Part I presents one concrete interpretation of the shift based on the mechanism proposed by Lieberman

*et al. *

[2]. However, it is possible to obtain similar interpretations for other mechanisms, such as short-range order. The principal assumption of the model is that the material has a few energetically preferred states, with each preferred state characterized by a preferred strain and shift.

Second, the relaxation of the shift is assumed to be much slower than the attainment of elastic equi- librium, so that kinetics is dominated by the shift relaxation. Third, the shift evolves by gradient-flow kinetics on this multi-welled energy. We write down equations based on these ideas and solve them given the initial state, applied load and temperature history.

All the parameters in our model are easily determinable and held fixed during the simulations.

Further, our model does not incorporate any

*ad hoc *

criterion to obtain the hysteresis or its evolution.

They all follow from the basic equations.

In Section 6 of Part I, we show that the results of our simulations compare favorably with the exper- imental observations of Lieberman

*et al. *

[2]. Our model is able to capture all the qualitative features of the wide range of experiments. Further, we also found quantitative agreement wherever such a comparison was possible; unfortunately, given the nature of the available experimental data, detailed quantitative investigation of the model was not possible. In Section 2, we simulated some experiments on the stabilization of martensite qualitative and quantitative

We can therefore agreement. conclude that to find good the simple statement of Christian, together with some easily measured material constants, is sufficient to predict many aspects of the behavior of these alloys.

In Section 3 of this part, we have proposed new experiments for two purposes. The first is to provide definitive quantitative tests for this model. The second and more important purpose is to use this model to further investigate the mechanisms respon- sible for these relaxation mechanism.

*Acknowledgements-We *

gratefully acknowledge many use- ful and colorful discussions with David Lieberman. Part of this work was conducted when K.B. and P.J.S. held post-doctoral positions at the Courant Institute. This work was partially supported through grants from the AFOSR

(KB, PJS:90-0090 at Courant, KB:F49620-95-1-0109 at

Caltech, RDJ:91-0301) ARO(KB:DAAL03-92-G-0011 at

Courant, PJS:DAAH04-95-1-0100 at

Courant),

DOE(PJS:W-7405-ENG-36 and KC-07-Ol-Ol), NS-

F(RDJ:DMS-9505077, PJS:DMS-9402763 at Courant), and

ONR (KB:N00014-93-1-0240 at Caltech, RDJ:N/N00014-

95-l-l 145 and 91-J-4304).

REFERENCES

1. Bhattacharya, K., James, R. D. and Swart, P. J.,

*Acta *

*Mat. *

2. Lieberman, D. S., Schmerling, M. A. and Karz, R. S., in

*Shape Memory E#ect in Alloys, *

ed. J. Perkins,

Plenum Press, New York, 1975, pp. 203-242.

3. Murakami, Y., Morito, S., Nakajima, Y., Otsuka, K.,

Suzuki, T. and Ohba, T.,

*Mater. Lett., 1994, 21, 275. *

*4. *

Christian, J. W.,

*Metall. *

Trans.

*A, *

1982, 13A, 509.